Chapter 3: Interfacial properties in tunnel junctions based on complex oxides
4. Ferroionic induced interfacial superconductivity in tunnel junctions
In order to study the role of oxygen vacancies in interfacial properties of tunnel junctions, we fabricated multiferroic tunnel junctions based on the previous heterostructure, but replacing the top LSMO by a LSCO layer, which is a system that can act as an oxygen vacancies reservoir. We propose a strategy to arrive at a reduced complex-oxide phase in LSCO by exploiting the formation and migrating of oxygen vacancies in a ferroelectric tunnel junction as in a topotactic reaction [20,22,25,27,28]. As introduced before, we fabricated asymmetric tunnel junctions with the structure STO(100)//LSMO(30nm)/BTO(4.4nm)/LSCO(10nm), forming micron-size pillars combining optical lithography and ion milling techniques.
The transport across the ferroelectric barrier shows TER, which we are going to study at 100K. The procedure was to apply a ‘writing voltage’, VWrite, in a hysteretic sequence recording the resistance measured at a low voltage (VRead=10mV) between write voltages. Figure 3.21 shows an electroresistance loop of the sample, where one can see two stable resistance states in the system as a function of the applied voltage. A high resistance state for negative voltages, and a low resistance state for positive voltages. The Tunneling Electroresistance (TER) was calculated, giving a large value of 105 %. These enormous values of TER have been obtained in asymmetric tunnel junctions composed of very different materials . That is because ER has been attributed to asymmetries in the screening of the polarization charges by the two electrodes of the tunnel junction . However, in our case, this cannot be the reason of the large electroresistance, because here the two electrodes, LSMO and LSCO, are expected to have similar screening lengths. Since LSCO is an oxygen vacancies reservoir, the switching of oxygen vacancies, combined with the ferroelectric polarization switch) may be responsible for the ER effect.
In the electroresistance cycle we can appreciate a gradual resistance increase at positive voltages just before the positive voltage switch, and also an equivalent depression before the negative voltage switch. These onsets correspond to a gradual displacement of oxygen vacancies across the BTO. However, the abrupt switches cannot be explained with oxygen vacancies movement only. Thus, ferroelectric polarization switches concurrently with oxygen vacancies [65,66].
79 Differential conductance measurements were taken at the two resistance states in order to study the low voltage dependence, as it is proportional to the shape of the tunnel barrier (Figure 3.22). The curves display a parabolic behavior, which is characteristic of tunneling transport. We appreciate that a strong voltage asymmetry appears in the low resistance state, which is not present in the high resistance state, denouncing a deep change in the shape of the tunnel barrier.
In order to study the evolution of the tunnel barrier effective shape, differential conductance curves were analyzed with the Brinkman-Dynes-Rowell model (BDR)
Figure 3.21: Electroresistance loop measured at 100K. The yellow arrows indicate the direction of the ferroelectric polarization for each resistance state of the systems.
Figure 3.22: Points: Differential conductance vs. voltage measurements taken at 100K in the high (left) and low (right) resistance states. Lines are fits to the Brinkmann, Dynes and Rowell model.
for a trapezoidal tunnel barrier . In this method, and assuming WKB approximation , which implies that the band structure of the M-I-M system varies slowly compared to the electron wavelength, the conductance is given by:
Where ϕ is the average barrier height, Δϕ=ϕ2-ϕ1 is the barrier asymmetry,
𝐴0 = 4(2𝑚)1/2𝑑/3ħ, and (32)
𝐺(0) = (3.16 · 1010· 𝜑1⁄2/𝑡)𝑒(−1.025·𝑡·𝜑1⁄2) (33) where t is the barrier thickness in Å and the voltage in volts.
Table 1: Tunnel barrier shape parameters obtained in the BDR fitting to the differential conductance curves in the high and low resistance states of the tunnel junction
Fits to this model are present in Figure 3.22 as lines in the differential conductance plots. These fits quantify the height and the asymmetry of the tunnel barrier. The data obtained and the estimation of the barrier shapes are in Table I.
In the HRS, the barrier thickness obtained is 4.5nm, in very good agreement with the nominal thickness of BTO, which is 4.4nm. The barrier height is 210 meV, with a small asymmetry (Δϕ=54 meV). On the other hand, in the LRS, a much larger average barrier height was obtained, ϕ=622 meV, with also a strong asymmetry (Δϕ=430meV). The barrier thickness is t=1.8nm, much smaller in this state. These changes in the barrier dimensions account for the large electroresistance found. In fact, they demonstrate that the oxygen vacancies ionization is driven by the ferroelectric polarization switching, outlining the role of the ferroionic coupling in a mixed electrochemical-ferroelectric state . The height of a tunnel barrier is determined by the distance from the Fermi level to the edge of the conduction band.
In BTO, at equilibrium, the Fermi level lies above the donor level of oxygen vacancies, which is 0.4 eV below the conduction band edge. These oxygen vacancies should be weakly ionized at the temperature of the experiment in the HRS,
State ϕ (meV) Δϕ (meV) t (nm) Barrier shape
HRS 210 54 4.5
LRS 622 430 1.8
81 explaining the low barrier height in this state. On the other hand, a strong increase is produced in the barrier height when the system switches to the LRS, this, together with the strong asymmetry, indicates a much stronger ionization of the oxygen vacancies at the bottom interface than at the top interface. The difference in the ionization between the two interfaces is due to the ferroelectric polarization and occurs to screen polarization charges. When the polarization is pointing up, the oxygen vacancies generated at the bottom interface get ionized, donating electrons to the top interface to screen the polarization charges. That in turn reduces the barrier width. For negative electric fields (FE polarization pointing down), the oxygen vacancies abandon the interface, and the screening is carried out by the holes of the LSCO. This yields a more symmetric tunnel barrier. These two states are schematically presented in the Figure 3.23.
The temperature dependence of the transport properties was also measured for the two resistance states. Current vs. voltage and differential conductance measurements were taken between -100mV and +100mV in a temperature range between 5K and 200K. The IV curves (Figure 3.24 left panels) show a non-linear dependence which is more pronounced at low temperatures. This is the typical behavior of a current across a tunnel barrier. We can see that at the LRS, the curve is almost linear, and this is in agreement with the thinner barrier found in this state.
At low temperatures, the differential conductance plots (g(V)) display a conductance suppression near low voltages that suggests the opening of a temperature dependent gap (Figure 3.24 right panels). This gap seen to be present in the two resistance states of the system. In order to clarify the dimensions of the gap in both resistance states, the conductance plots were normalized to their value at 40mV (G=
(g)/(g(40mV))) and corrected for the normal state conductance by dividing each curve below 100K by the 100K one (G/GN(100K)). When we do this, a clear gap
Figure 3.23: A: Scheme of the screening charges distribution in the junction when the ferroelectric polarization points down. The oxygen vacancies inside the BTO are neutralized and the screening is performed by the holes inside the LSCO. B: When the polarization points up, the oxygen vacancies get ionized inside the BTO and their electrons screen the polarization charges at the top interface.
emerges in the HRS, resembling a superconducting gap (Figure 3.25 left panels). In the HRS (upper panel) the gap persists up to 80K and takes values of 50 mV, which are characteristic values of superconducting cuprates. The gap still appears in the LRS, but is shallower, reaching values of 30 mV of width, and closes at 40K (lower panel). The right panels of Figure 3.25 show the contour plots of differential conductance, which illustrate the differences of the gap features in the two resistance states. We can conclude that the interface superconducting state can be switched on and off by applying an electric field. In the HRS even appears quasiparticle peaks around 40 meV (Figure 3.26).
This gap has been observed in three more samples, one of them with silver instead of gold as top electrode (See appendix 2), but in another sample, with lower conductance in the initial state, a conductance enhancement is present at small bias, instead of a conductance suppression (Figure 3.27). The conductance enhancement remains until temperature exceeds 60K and until voltage exceeds 40 mV. This behaviour is characteristic of the Andreev reflection in a metal/superconductor junction, and therefore strongly suggests the presence of a superconducting state at the interface [68,69]. In summary, switching between HRS and LRS, driven by the application of an electric field, modulates the superconducting properties of the LSCO interface.
Figure 3.24: Current vs voltage (left panels) and differential conductance vs voltage (right panels) curves as a function of temperature when the sample is in the HRS (upper panels) and in the LRS (lower panels).
83 It is possible to analyse this phenomenon in the frame of the Bloder-Tinkham-Klapwijk (BTK)  theory for superconductor/metal junctions (Figure 3.28). The fittings were performed by Kevin Seurre in the group of Javier E. Villegas in Unité Mixte de Physique, CNRS, Thales, Université Paris-Saclay. This theory explains the special features of conductance spectra associated to the superconducting gap (Δ) in terms of a Z parameter, which measures the strength of the junction’s barrier. As Z increases, the junction transparency reduces. The transparency is defined in terms of the mismatch of Fermi velocities at the normal and superconductor sides; also, it can be defined as the strength of the oxide barrier in a tunnel junction.
The used fit for both resistance states is a BTK modified version for d-wave superconductors extended to the case of c-axis tunneling [71,72]. According to the peak structure of the system, it can be interpreted as a spectral convolution of the d-wave quasiparticle DOS, which gives a V-shaped gap broadening and the quasi-2D normal-state DOS, which has a logarithmic singularity near the Fermi level. The conductance expression is as follows:
Figure 3.25: Left: Differential conductance curves normalized to the 100K curve for ferroelectric polarization pointing down (upper panel) and up (lower panel). Color code reflects temperature increase as shown in the left arrow. Right: Contour plots showing the emergence of a gap and its evolution with temperature for ferroelectric polarization pointing down (upper panel) and up (lower panel).
𝜎̃𝑠(𝐸, 𝜃) = 16(1 + |𝛤+|2) cos4𝜃 + 4𝑍2(1 − |𝛤+𝛤−|2) cos2𝜃
|4 cos2𝜃 + 𝑍2[1 − 𝛤+𝛤−𝑒(𝑖𝜑−−𝑖𝜑+)]|2 (34)
Where Z is the barrier strength, Γ±= (𝐸
∆±) − √( 𝐸
− 1, and 𝑒(𝑖𝜑±)= ∆±⁄|∆±|.
This expression represents the phase of the pair potential experienced by an Andreev-reflected electron (or hole) propagating at an angle θ relative to the junction normal. The tunneling current is also proportional to a parameter β, which in case of an interface in the Normal/Insulator/Superconductor limit, is rather small.
In addition to the bare extended BTK model, broadening effects were considered, in particular the effect of quasiparticle lifetime [73,74], which can be quantified by
Figure 3.26: Enlarged view of the normalized differential conductance of the junction from figure 3.25 left upper panel. Quasiparticle peaks are observed at low temperatures.
Figure 3.27: Left: Zero bias peak present in another junction at low temperatures and bias. The peak persists until 60K. At high voltages (right) the behavior reminds of a typical tunnel junction.
85 means of a phenomenological parameter Γ. As seen in the Figure 3.28, the data are in good correlation with the BTK theory for the state with the enhanced superconductivity, whereas shows a symmetric behavior which does not correspond to the real measurements for the depressed-superconductivity state. This difference may be due to the fact that the BTK theory applies only for Normal/Superconductor interfaces. The values obtained from the BTK fitting are summarized in the Table 2.
If this study is carried out at several temperatures, one can obtain the temperature evolution of the superconducting gap. These plots show familiar behaviour  as shown in the inset to Figure 3.28b. In the high resistance state the gap closes at a temperature slightly exceeding 70K, while in the low resistance state it closes below 50K. Within the BTK theory, this may be interpreted as Z being larger in the in the HRS than in the LRS in agreement with our results.
Figure 3.28: Manifestation of superconductivity in the high and low resistance states (respectively HR and LR). a) Normalized conductance of the HR state (scatter) and the extended BTK-simulation (line)  with Z=30 for T=13,24 and 52K. b) Normalized conductance of the LR state (scatter) and the extended BTK-simulation (line) with Z=1.7 for T=5,10 and 30K. c) Extracted value of the superconducting gap for the two states (scatter) and their fit (line)  to determine an estimate of the critical temperature Tc. For the HR state, Tc≈71K and for the LR state, Tc≈48K.
Table 2: Parameters obtained from the BTK fitting to the differential conductance measurements.
T=5K Z Δ Γ
HRS 22 10.5 8
LRS 2.42 22 22
A fitting was performed to deduce the Tc of the superconducting state for the high and low resistance states (Figure 3.28c) as done in . Here we can estimate a critical temperature of Tc=70K for the HRS, which is very similar to that in YBCO, and Tc=50K for the LRS.
The sample with a conductance enhancement at low voltages has been fitted with the BTK model, as can be seen in Figure 3.29. This zero bias peak appears in d-wave superconductor/metal interface where the superconducting parameter makes an angle of 45o with the interface (α=π/4) . The change of sign of the order parameter for the incident and reflected quasiparticle results in the formation of quasiparticle bound states at the interface between the superconductor and the metal. This resonant zero energy bound states dominate the tunneling process at low bias and gives rise to the peak at zero bias. Such a geometric tunneling configuration requires that the epitaxial growth is locally modified to expose the nodes of the order parameter to the tunneling cone. A situation favored by the rather high density of stacking faults observed in the high resolution microscopy images of the heterostructure in Figure 3.7b, which probably result from the transfer of oxygen vacancies. The finding of the two different features, the gap-like behavior and the zero bias conductance peak in this system strongly supports the existence of a superconducting state at the BaTiO3-cuprate interface which is modulated by the resistive switching.
The transfer of OV from the cuprate to the ferroelectric produces structural modifications besides the doping effect and are crucial for the stabilization of the superconducting state. For example, it can be observed in the microscopy image (Figure 3.7b) that the buckling of the lattice planes induced by oxygen vacancies is suppressed, indicating that the depletion of OV is accompanied by structural changes. The OV are known to be the origin of the lack of superconductivity of the LSCO cuprate. It has been proposed that their electron doping field compensate the effect of the holes introduce by the Sr doping, and because of that, the CuO2 planes never reach the doping level necessary to start superconducting. Furthermore, the arrays of oxygen vacancies lining up along a and b directions of the unit cell break the necessary connectivity of CuO6 octahedra keeping the 3D transport metallic, although anisotropic, but hindering the nucleation of superconductivity .
OV transfer across the junction produces a strong modification of doping at the cuprate interface, which is also modulated by the coupled switching of ferroelectric polarization and oxygen vacancies. If the 3.9 oxidation state over the whole BTO barrier is caused by the transfer of oxygen vacancies from the (whole) 10 nm thick cuprate layer, this would produce a hole doping of 6.6 1020 cm-3 which will be
87 modulated at the interface layer by ferroelectric field effect. It is precisely in the high resistance state where the larger gap is observed, that the cuprate will be strongly hole doped by the depletion of oxygen vacancies and the screening of the negative (down) polarization charges (Figure 3.23). As discussed above, these vacancies transferred to the BTO are weakly ionized in a way dictated by the ferroelectric polarization, and consequently the barrier remains insulating. On the other hand, in the low resistance state, with a smaller gap, oxygen vacancies have been partially swept to the cuprate and polarization is pointing up, what favors less hole doping of the interface. Now polarization is partially screened by the oxygen vacancies remaining in the barrier (what increases their ionization) and thus contribute less to electron doping of the cuprate.
In summary, we have found fingerprints of superconductivity at the interface between a non-superconducting cuprate and a ferroelectric barrier in a tunnel junction. Both the energy size and the temperature range of the gap suggests a high critical temperature of 80 K in a cuprate where superconductivity had never been found before. We propose that the transfer of oxygen vacancies from the cuprate interface to the titanate barrier triggered by the modulation of the lattice expansion at both sides of the interface, plays a major role on the stabilization of the superconducting phase. In addition, the coupled switching of ferroelectric
Figure 3.29: Normalized conductance of one particular sample and a simulation with the extended BTK method for d-wave superconductors. This zero bias conductance peak is typical of d-wave superconductor/metal interface where the superconducting order parameter makes an angle of 45°
with the interface . This peak results from the formation of quasiparticle bound states at the interface between the superconductor and the metal.
polarization and oxygen vacancies produce a strong doping modulation at the interface layers resulting from the combined effect of the doping field of the oxygen vacancies and the field effect to screen the ferroelectric polarization.